In-Situ Observation and Acoustic Emission In-Situ Observation and Acoustic Emission Monitoring of...
Embed Size (px)
Transcript of In-Situ Observation and Acoustic Emission In-Situ Observation and Acoustic Emission Monitoring of...
In-Situ Observation and Acoustic Emission Monitoring of the Initiation-to- Propagation Transition of Stress Corrosion Cracking in SUS420J2 Stainless Steel
Kaige Wu1,+, Fabien Briffod1, Kaita Ito2, Ippei Shinozaki3, Pornthep Chivavibul1 and Manabu Enoki1
1Department of Materials Engineering, The University of Tokyo, Tokyo 113-8656, Japan 2Research and Services Division of Materials Data and Integrated System, National Institute for Materials Science, Tsukuba 305-0044, Japan 3Materials Department, Research Laboratory, IHI Corporation, Yokohama 235-8501, Japan
In this work, acoustic emission (AE) monitoring was correlated with in-situ optical microscopy observation and electron backscatter diffraction (EBSD) measurements to investigate the evolution of a single stress corrosion crack in SUS420J2 stainless steel subjected to chloride droplet corrosion. A single dominant crack evolution was observed to transition from a slow initiation of active path corrosion-dominant cracking to a rapid propagation of hydrogen-assisted cracking. The initiation-to-propagation was concomitant with a significant increase in the number of AE events. In addition, a cluster analysis of the AE features including traditional waveform parameters and fast Fourier transform (FFT)-derived frequency components was performed using k-means algorithms. Two AE clusters with different frequency levels were extracted. Correlated with the EBSD-derived kernel average misorientation (KAM) map of crack path, low-frequency AE cluster was found to correspond with the location of plastic deformation in the propagation region. High-frequency AE cluster is supposed to be from the cracking process. The correlation between AE feature and SCC progression is expected to provide an AE signals-based in-situ insight into the SCC monitoring. [doi:10.2320/matertrans.MT-MAW2019004]
(Received May 16, 2019; Accepted June 20, 2019; Published July 26, 2019)
Keywords: stainless steel, stress corrosion cracking (SCC), pitting, plastic deformation, acoustic emission (AE), electron backscatter diffraction (EBSD)
Stress Corrosion Cracking (SCC), caused by the syner- gistic interaction of corrosive environment and mechanical load, is an important threat to stainless steels. Considering the widespread use of stainless steels, SCC has been a primary cause of many failures of metallic structures and components in a wide range of industries.1) Thus, the reliable assessment of the service life of the exposed components and structures requires the accurate prediction of initiation and propagation of SCC.
It is clear that SCC requires contributions from both chemical and mechanical factors. Parkins2) firstly put forward the concept of “stress corrosion spectrum” to support a continuous spectrum of SCC mechanism. It is suggested that SCC is predominantly controlled by a changing dominant factor from electrochemical to mechanical depending on the SCC progression. Figure 1 shows a schematic elucidation of a three-stage model for SCC progression which was rearranged based on the references.24) Despite its complex nature due to combined metallurgical, mechanical and environmental effects, SCC in most cases begins with the early localized corrosion4) or mechanical defect sites like pitting, intergranular attack (IGA), scratches, or other pre- existing flaws, subsequently develops as a short crack with slow propagation, to finally reach the long crack regime eventually leading to the ultimate failure of the component. The SCC development in the initiation regime is often perceived to be slow and long term and can largely determine the overall life of an exposed component.5,6) Therefore, an in-situ monitoring of the initiation-to-propagation transition is greatly significant in the lifetime estimation of SCC.
In general, the initiation and propagation of SCC are strongly affected by the electrochemical conditions and the local stress/strain state at the crack tip, and cannot be directly and integrally estimated via traditional electrochemical methods7) or mathematical based models8) given the difficulties to obtain the experimental input parameters. Acoustic emission (AE) method, a nondestructive testing (NDT) method based on the recording of elastic waves, is known to be highly sensitive to local phenomena such as chemical reactions and physical changes. AE method has long been used to study the steel corrosion like pitting corrosion and SCC.918) Some of the registered sources of AE signals in literature include pitting,913) hydrogen bubble evolution,914) dislocations motion during plastic deforma- tion,15) cracking of oxide/corrosion products,14,16) falling-off of surface grain,14,16) generation and propagation of cracks.13,1518) However, so far no attention was paid to combining in-situ observation and AE monitoring for the transition identification during SCC progression, which is the primary concern of the present work.
However, the accelerating SCC tests, recommended by ASTM G129,19) ASTM G36,20) or NACE TM0177,21)
basically require the immersion of specimens into a bulk solution at an elevated temperature which is challenging to facilitate AE experiments and in-situ observations. In the present work, a chloride droplet SCC test was improved with the smooth U-bent SUS420J2 stainless steel specimen in humidity to trigger a single crack evolution, thus accom- modating the experimental aim. Moreover, electron backscatter diffraction (EBSD) analysis of the crack path was correlated with in-situ observation and AE behavior in time evolution so as to track the features in relation to the initiation and propagation of SCC.
+Corresponding author, E-mail: [email protected]
Materials Transactions, Vol. 60, No. 10 (2019) pp. 2151 to 2159 ©2019 The Japan Institute of Metals and Materials
2. Experimental Procedure
2.1 Material and specimen A commercial SUS420J2 stainless steel (provided by
Kusayama Unique Special Steel, Japan, C: 0.32mass%, Si: 0.45mass%, Mn: 0.54mass%, Cr: 13.39mass%, Ni: 0.09 mass%, P: 0.031mass%, S: 0.005mass%, Fe: bal.) was used in this study. To improve the corrosion susceptibility, the steel was first treated at 600°C for 1 h and 800°C for 1 h to precipitate the carbides. It was then annealed at 1010°C for 2.75 h and quenched in Argon air cooling. The obtained mechanical properties of the steel were characterized by a 0.2% proof stress of 1201MPa, an ultimate tensile strength (UTS) of 1679MPa, an elongation of 0.9% and a Vickers hardness of 611. The specimen was machined from the bulk steel after heat treatment with a dimension of 170.0mm (L) © 6.3mm (W) © 1.5mm (T) and finally polished up to 0.05 µm Al2O3 slurry for a mirror finish. Figure 2 shows the microstructure of the steel specimen after being etched using Viella’s reagent for 10 seconds, indicating the martensitic lath with visible prior-austenite grain boundaries. The average gain size was determined as 22.8 µm. Circular and elongated undissolved carbides were observed within martensitic grains, especially near prior-austenite grain boundaries. Further energy-dispersive X-ray spectroscopy (EDX) mapping confirmed the carbides with enrichment in carbon and chromium and depletion in iron, indicating Cr-rich carbides. The specimen was intended to have low toughness, high residual stress and active corrosion path (i.e., grain-boundaries with segregated Cr-rich carbides) to facilitate the crack initiation.
2.2 SCC experiment and AE measurements To improve the reliability in extracting and interpreting the
AE signals, a localized SCC attack under a single chloride droplet accommodated with a continuous in-situ monitoring by digital microscope was designed with AE measurements. Figure 3 shows the experimental setup. The specimen was
bent and fixed in an experimental jig with a curvature radius of 125mm leading to a constant strain of 0.6% at the apex of the specimen surface. A 1µL droplet of 1.0mass% neutral NaCl solution was dropped in the center area of the specimen surface using a microliter syringe. The experimental apparatus was placed in a thermostatic bath (298K, 99 100% humidity) with pure water. The bath was covered with a transparent glass cap to allow in-situ observation using a digital microscope (VHX-5000, Keyence Corp., Japan). Simultaneously, continuous AE measurement was performed using a custom AE acquisition system developed in our group, CWM.22) Two high-sensitivity R-CAST sensor systems with a resonant frequency of 200 kHz (M204A, Fuji Ceramics Corp., Japan, 55 dB gain) were positioned 10mm and 30mm away from the droplet site to record the AE signals. A threshold of 27 dB and a 100 kHz high-pass filter (HPF) were used as thresholds to isolate AE events from the continuous waveform. Then the target signals were extracted
Fig. 1 Schematic diagram of a three-stage model for SCC progression. Rearranged based on Refs. 24).
Fig. 2 The microstructure of chemically etched specimen: (a) optical micrograph, (b) backscattered electrons (BSE) SEM image, and (c) EDX maps.
K. Wu et al.2152
by filtering out the noise outside the corrosion region using the source location method.
2.3 Cluster analysis of AE data A cluster analysis of the extracted AE data was performed
using K-means algorithm. To improve the classification of AE signals, the traditional AE parameters (i.e., amplitude, rise time, duration, counts+) together with the FFT frequency components from 102.5 kHz to 996.1 kHz with a resolution of 4.9 kHz were input as AE features into the k- means algorithm. All input data were first normalized with Z- score standardization method.23) Then principle componen